# abaqus-compaction and tensile damage in concrete constitutive

Post on 27-Nov-2014

264 views

Embed Size (px)

TRANSCRIPT

Compaction and tensile damage in concrete: constitutivemodelling and application to dynamicsNicolas Burlion, Fabrice Gatuingt, Gilles Pijaudier-Cabot *, Laurent DaudevilleLMT-Cachan, ENS Cachan/CNRS/Universit e P. et M. Curie, 61 avenue du Pr esident Wilson, F-94235 Cachan Cedex, FranceReceived 4 May 1998AbstractThe objective of this study is to develop a model for concrete with an emphasis on tension and compaction. Compaction of concreteis physically a collapse of the material voids. It produces plastic strains in the material and, at the same time, an increase of the bulkmodulus. The model is based on mechanics of porous materials, damage and plasticity. The computational implementation has beencarried out in the Lagrangian nite element code DYNA3D. In order to show the inuence of compaction, simulations of a splitHopkinson test performed on conned concrete and on a concrete rod submitted to an impact have been carried out. The examplesdemonstrate the importance of compaction during an impact, which has a tendency of strengthening the concrete structure. 2000Elsevier Science S.A. All rights reserved.1. IntroductionIn a concrete structure subjected to a shock or to an impact, for instance a concrete slab, the material issubjected to various states of stresses which yield dierent failure modes. Near the impactor, severe hy-drostatic compression is observed. This state of stress produces irreversible compaction of the material.Farther from the impact location, the connement stresses decrease and the material experiences com-pression with a moderate triaxial state of stress. Finally, compressive wave reection may occur and canresult in a tensile wave which will interact with compressive waves and produce spalling, i.e. tensile crackinginduced by wave interaction. Computational analysis of concrete and reinforced concrete elements sub-jected to this type of loading history requires the implementation of a constitutive relation capable ofcapturing the major features of the material response under such loads: tensile cracking, compressionfailure and the eect of connement on the ultimate stress, and nally compaction which induces an in-crease of the tangent and elastic stiness of the material, an increase of the wave speed and consequentlysubstantial modications of wave interactions which may aect tensile cracking and failure. Fig. 1 showsexperimental results from [6] on which the hydrostatic stress has been plotted versus the volumetric strainfor two dierent loading histories: triaxial hydrostatic compression and oedometric compression inspiredfrom the testing procedure devised by Bazant et al. [3] (i.e. with zero, or quasi-vanishing, transverse strains).Looking at the material response and from a phenomenological point of view, constitutive models shouldincorporate irreversible plastic strains, an increase of stiness due to compaction of concrete, and materialdamage due to progressive cracking in tension which does not occur in the experimental results shown inFig. 1. Furthermore, these experimental results show that it is not possible to separate the deviatoric andhydrostatic responses of the material, as opposed to the assumption commonly used in most materialwww.elsevier.com/locate/cmaComput. Methods Appl. Mech. Engrg. 183 (2000) 291308*Corresponding author.0045-7825/00/$ - see front matter 2000 Elsevier Science S.A. All rights reserved.PII: S 0 0 4 5 - 7 8 2 5 ( 9 9 ) 0 0 2 2 3 - 6models for impact problems. Would the hydrostatic and deviatoric responses be uncoupled, the two curvesin Fig. 1 would be exactly the same.Except maybe for the microplane model which is derived from dierent modelling principles [1,2]),phenomenological damage or plasticity models are usually capable to describe correctly the behaviour ofconcrete if one of the principle strains is positive and more generally in biaxial situations (see e.g. [21,10]).Most of these models are not capable, however, to capture the eects of severe compaction because of twodiculties:1. Plastic strain growth under an hydrostatic state of stress and material stiening (loading and unloadingstiness). This is due to the plastic/damage loading functions which should be closed on the hydrostaticaxis, e.g. with a cap (see e.g. [20]).2. Theoretical diculties which prevent a decrease of damage, and thus an increase of elastic stiness.From the viewpoint of thermodynamics of irreversible processes, damage cannot decrease in a closedsystem, unless another dissipative mechanism occurs at the same time which results in a positive globaldissipation rate (which would be negative otherwise).In this contribution, we present a model which has been developed, keeping in mind these two di-culties. The originality of the model compared to the approaches based on cap models in plasticity is thedescription of the variations of the material elastic stiness. The degradation of the elastic moduli is de-scribed in the model by two damage scalars: a tension damage variable and a compression damage variable.Tension damage is controlled by the positive elastic strains. In order to capture the evolution of plasticstrain we use a modied Gursons yield function with associated ow rules [15,23]. The evolution of thevolume fraction of voids entering in the Gursons yield function is directly related to compression damage.When it decreases, it produces an increase of the material stiness and therefore a decrease of materialdamage. Hence, the evolution of compression damage and plastic strain are entirely coupled. Section 2presents this constitutive model and its calibration from experimental results. In Section 3, the imple-mentation of this model in the nite element code DYNA3D is proposed. Finally, computations on testcases which exhibit the major properties and characteristics of the model are presented in Section 4. We doFig. 1. Experimental hydrostatic and oedometric test results (after Burlion, 1997).292 N. Burlion et al. / Comput. Methods Appl. Mech. Engrg. 183 (2000) 291308not intend to deal here with thorough comparisons with experimental results, but rather to exhibit theinuence of its major characteristics on the response of small structures in transient dynamics.2. Constitutive modelIn the following, we will use the small strain assumption and the standard decomposition of strain in-crements into elastic and plastic parts:deij(xY t) = deeij(xY t) depij(xY t)Y (1)where eij(xY t) are the total strain components, eeij(xY t) are the elastic strains, and epij(xY t) are the irreversiblestrain components. We are going to present rst the elastic-damage part of the model. Plasticity will beadded later and coupled to the foregoing damage model.2.1. Damage modelWe focus in this section on the relationship between the elastic strain tensor and the stress tensor. Thereare two mechanisms which induce a variation of the elastic moduli of the material: The rst one is microcracking. In tension, where we expect that the plastic strains are very small com-pared to those in compression, the material nonlinear response is due almost solely to microcrackgrowth. As we will see in Section 2.2, tension damage will be considered to be controlled by positivestrains which produce microcrack opening and microcrack growth. In compression, and more specically for states of stress where the connement prevents microcrackopening, the other damage mechanism is the crushing of the cement or mortar matrix in concrete. It in-duces a variation of the volume fraction of voids which will later be considered to be driven by the irre-versible plastic strains.An important issue is now the type of damage variables to be used is whether the directionality ofdamage (understood here as microcracking and variation of void volume fraction) is important or not.Damage due to the variation of the volume fraction of voids, later on denoted as compression damage, caneasily be considered to be an isotropic phenomenon. From a physical point of view, it is very clear,however, that microcracking in tension is geometrically oriented. Microcracks develop in planes which areperpendicular to the applied stress. One approach would be then to consider that tension damage growthinduces in this case elastic orthotropy. Such models have been devised in the literature, among others, bySidoro [26], Chaboche et al. [7], Dragon and Mroz [9], Berthaud et al. [4], Valanis [28]. Recent resultsby Fichant et al. [11], however, have shown that in situations where material failure is essentially controlledby one-dimensional extensions, scalar damage models provide numerical predictions at the structural levelwhich are very similar to orthotropic damage models. In fact, damage induced anisotropy was found to beimportant when the material is subjected to multiaxial extensions which induce damage growth, and alsowhen the strain history applied to the material is severely non-radial.In view of the complex

Recommended